Selection of Structural Materials for Extreme Loads Environments
THE SOCIETY OF NAVAL ARCHITECTS ANO MARINE ENGINEERS
One Wwld TradeCenter,
Selection of Structural Materials for Extreme
Robert H. Sterne, Jr., Lukens Steel Co., Coatesville, PA
A variety of ferrous and nonferrous metals are used in the Con.
struction of large ocean qoincj
The purpose of this paper
is to generally review a“ailable
structural materials and highlight
characteristics which are critical
in extreme loads environments.
Specific material properties are
reviewed in 1ight of the evolution
of manufacturing technology with resultant improvements in such factors
as strength, notch toughness, and
The scope of the paper includes
treatment of steel, al”min”m, copper
1 alloys and titanium.
Specifications which are currently
available for designer’s use are
reviewed as a function of yield a“d
Measuring 60 feet i“ length, the
Codorus drew only six inches of water.
Those first hull plates measured 1/4,,
by 24,7x 37s8,while the boiler itself
used 3/8” thick plate (Figure 2) .
A search of the historical
records shows that the first metalhulled ship built in the USA was
launched in 1825. The COdOrUS WaS
plated with iron rolled by the
Brandpuine Iron and Nail Factory in
built in York, Pennsylvania and
steamed “p the Susquehanna River on
her maiden voyage (Figure 1) .
no hull steel specification --
of that cane later.
Following the Codorus , a long
line of larger vessels were built,
first with iron plated hulls, and
later with steel. Through the nine teenth century and into the twentieth,
riveting was the predominate method
of joining metal plate toqether to
form the structure.
●Tensile and Yield Strength
The American Bureau of Shipping
(ABS) was incorporated in 1862, and
began the technical process of writing
rules for shipbuilders and designers.
The 1980 rules (1) referenced in this
paper apply to ocean going “essels 61 m
(200 feet) and o“er in length.
The sort of loading anticipated
will dictate to some degree the
strength le”el of the material.
size of the structure and its response
to the sea state is another important
factor . Within the confines of other
desired properties , economics will
ha”e a bearing.
Rules for aluminum vessels were
last published in 1975. In addition,
a number of ABS publications describe’
Rules for Barges (3), Floating Dry
Docks (4), Underwater Systems and
Vehicles ‘5), and Great Lakes Ore
Subsea str”ct”res are subjected
both to compressive and tensile loads ,
but must also be designed with
buoyancy in mind, where higher
strength to weight ratio materials
have an advantage.
often is the key characteristic.
Further, ASTM ‘7) has adopted ABS
materials Specificat ions, and API
publishes steel specifications (8) for
offshore drilling platforms . And this
is just for the USA. Other countries
In short, selection of the proper
le”el of yield or tensile strength
depends on the integration of the
other design criteria into the particular hull or other structure .
It 9s ob”io”s
Lamellar Tearing Resistance
A separate set of ABS rules
exists for Building and classing Offshore Mobile Drilling Units (2), originally published in 1968, and revised
in 1973 and in 1980.
been described that there is a high
degree of complexity to both shipbuilding rules and the materials
specifications that are permitted for
Today, the “ast majority of
metals used in marine stjmct”res are
Coupled with the
need for forming, tensile ductility
is a necessary ingredient in any metal
used for hulls, platform legs, or for
the pressure hull of submersibles.
However , this symposium has been
assembled to address extreme loads.
From the standpoint of materials
application, extreme loading can be
addressed in light of the following
characteristics which can be written
into the specification (Figure 3) .
Shipyard welding conditions are
usually far from ideal, with little
Metals used, thus, should
have a high le”el of tolerance to
these varied conditions.
Ship Structure Committee project is
directed at impro”ing the weldability
Of ship hull steels of 50 KS1 yield
strength ‘g) at high heat inputs.
Tolerance for fabrication errors
is another desired characteristic.
recent Ship Structure Committee report
(lo) puts further definition on this
High strength (> 60 KS1 minimum
Y.S .) and non-ferrous materials qenerally require environment control in
the fabrication pr,Jce~~.
Brittle fracture (Figure 4) has
been recognized as probably the leading cause of ship materials failures
Development of more sophisticated
test methods has continued in the
twenty years. The Fracture Analysis
Diagram (Figure 7) approach ad”anced
since World War II (11 and 12) . The
amount of materials research and
development work done to sol”e this
Problem is staggering, and has result.
ed in numerous improvements in specifications through the adoption of both
steelmaking and testing safeguards.
U.S. Naval Research Laborato~
Notch toughness--the ability of
metals to resist brittle fracture -was recognized as an essential materials characteristic in the 1945-1950
ha”e been gradually made since that
time requiring testing to establish a
minimum level of notch toughness in
certain critical hull areas.
Charpy V-notch test has been used aS
the primary qualification test (Figure
5 and Figure 6) .
This has allowed designers to specify
levels of “etch toughness that can
correlate more closely with their
expectations of the loading which the
marine structure will experience.
by Pellini and co-workers relied on the
Drop Weight Test--a ,,go,no-go’, test
that established a lower temperature
boundary below which steel lates were
considered to be brittle (137 (Figure 8) .
Improvements in manufacturing
methods such as vacuum degassinq, desulf”rization and consumable remeltinq
have allowed the designer to specify
higher levels of “etch toughness .
Shown here are some of the available
manufacturing methods to produce higher
quality levels through melting
(Figure 10) .
g 30g 20lo-
Reference 13 more completely explains
the concept of the fracture analysis
diagram and its application to ship
The dynamic tear test was developed at the U.S . Naval Research Laboratory to provide a more quantitative
measurement of notch toughness, and to
overcome the deficiencies of the Charpy
V-notch test; i.e ., a relatively blunt
notch and a short crack run. Although
it is not currently used as an acceptance test, a reasonable correlation
has been established between dynamic
tear and the Charpy v-notch data (14)
(Figure 9) .
FATIGUE RES lSTANCE
inu it ies
which can act
as locus points for the initiation and
propagation of fatigue cracks . Such
discontin”ities may be d“e to design
(such as sharp hatch cormers) , result
from fabrication (such as weld cracks)
or be present in the material itself.
Selection of materials and welding procedures to improve fatigue resistance In”st, of course, be integrated
into proper design.
Recent improve ments in steel refining practices [15)
as well as microalloying practices have
better fatigue resistance under certain
conditions ; specifically with low
sulfur content (> 0.010%) and with
sulfide shape control (Figure 11) .
Fatigue Crack Growth Rate - A633 Grade C
RES lSTANCE TO LAMELL,AR TEARING
Numerous factors bear On
the solutions to lamellar tearing
(Figure 14) .
Lamellar tearing results when
metals are strained through the thickness. When cracking results, it
Usually is associated with non-metallic
inclusions , in a plane parallel to the
surfaces of the material
(Figure 12) .
● Qualj~ control
● Fabrication procedures
Experience has shown that material with good through-gage (Z direction) ductility is more resistant
to lamellar tearing (Figure 15) .
Such lamellar tearing can be found in
highly restrained welded joints , such
as in K-braces (Figure 13) in offshore
Minimum percentage reduction of area
in the Z direction is commonly speci fied, Current steelmaking practices
allow the production of products with
less than 0.010% sulfur (Figure 16)
The mechanical properties of these
grades ha”e changed little over the
last thirty years, but the chemical
analysis has been adjusted to improve
Moreover, nOrmaliz notch toughness.
ing--to further improve notch toughness--is required by ABS for Grades CS
and E for all thicknesses, and for
Grade D over 1.375”.
B, D and E at
temperatures between O°F and -40°F.
Note that rimmed steel--once commonly
used--is now prohibited except for
Grade A under 1/2” .
and with inclusion shape control
(Figure 17) .
40-60 KS 1 YIELD STRENGTH
ABS rules incorporate two levels
of strength which are generically similar, Grades H32 and H36 (Figure 19) .
Specifications have been developed
for ship steels in an evolutionary
manner as research and development
indicated the proper directions, based
on designers needs. These will be
addressed on the basis of increasing
30-40 KS1 YIELD STRENGTH
These are the ordinary strength
hull steels described by ABS and ASTM
A131 as Grades A, B, CS, D, E and DS.
All have 34 KS1 minirn”m yield strength
(Y,S.) and 58/71 KS1 “ltirnate tensile
OVER 60-100 KS I YIELD STRI?NGTH
These steels have either 45.5 KS1 or
51.O KS1 minimum Y.S. and 68-85 or
71-90 KS1 U.T.S.
An increasing number of carbon
and low alloy steels are available in
this strength range; all require
quenching and temper ing to de”elop the
required strength leve 1s . A “umber of
proprietary specifications are available as well, but will not be discussed
here (Figure 22) .
More careful control of chemical
analysis and manufacturing practice is
required for DR and EH including fine
grain practice, impact testing and
either controlled rollin~ or normalizing based on thickness.
In addition, several ASTM specifications are attractive for USe in
this strength range (Figure 20) . These
Quenched and Tempered
>60.100 K[$ ~.$,
ASTM High Strength Steels For
ASTM A537 Class1
ASTM A633 GradeA
ASTM A678 Grade A
ASTM A737 Grade A
ASTM A67B Grade C
75 KS]VS. to 3/4’(
70 KSIYS.>3/4 - ‘1-’l/2
65 KSIV.S.>1-l/2 - 2“
ASTM A724 Grade A
70 KSIVS. to 5/8”
75 KSIYS to 5JW
These grades ha”e notch toughness
certification available at temperatures as low as -75°F and are often
the most economic
based on strength/weight/price considerations.
latter steels can be produced with
toughness certification to -80°F in
certain grades and thicknesses (Fiyure
90 KSIto-1 -l/2°
OVER 100 KS1 Y.S .
Use of steels in this strength
range has been limited. Small submersibles have used RY130-140 to Mil-
to 2“ or hea”ier,
broader use of HY130.
Both PH15-7M0 .a”dPR17-4M0 precipitation hardening, high strength
stainless steels, have bee” used i“
hydrofoil struts . These materials
combine the advantage of high strength
and corrosion resis’ta”ce with good
Alloy steels likewise are available and have been used, not only in
military vessels, but also in a variety
of commercial ships with unusual design requirements (Figure 23) such as
the Glomar Explorer.
Chemical Requirements and Minimum
[email protected] Mm.. %
SJIdwr. Mm., %
Figure 24 shows quenched and
tempered alloy steels at 60-100 H81
Quenched and Tempered
A31w A5s43Class 1
70 K$JV.S,to 10”
80 KSIY.S to 8“
85 KSIY.3 to 8-10”
100 KSIY.S.to 5-6
100 KSIY.S to B“
100 KSIY,S.GDges Vaiy By
100 KSIY,S1 Grade 1-1/4 6“
(0,394,0,394)2,8(20) 1,9(13.5) 4,2(30)
These grades are C-Mn fine yrai”
steels in the O°F to –67°F range.
_l.TERIALS TO CONTAIN LIQUEFIED CARGOS
Below -67 ‘F, nick. 1 containing
fine grain practice steels are allowed
with nickel content increase from 2~A
to 9% as design temperatures drop to
-3200F. Auste”itic stainless steels
are permitted to -3200F, as is l“var,
a 36% nickel ire”. B209, Type 5083
aluminum alloy is.permitted to -320°F.
Ladings such as LPG, Propane and
LNG require special low temperature
steels, which are defined by the lMCO
Gas Code as a function of temperature
(Figures 25 and 26) :
ALUMINUM AND ALUMINUM ALLOYS
Ocean going uses of aluminum, with
several exceptions, have been confined
to LNG containment
a“d to deckhouses and some s“per St131Ct”reS Of U.S . Navy combatants .
Hydrofoil hulls are being fabricated from aluminum plate both for
commercial and military service . Here,
weight is a major design consideration.
Primary emphasis has bee” placed
on steel since it is the most widely
used material of construction for
large ocean going ships.
COPPER ANC COPRONICKEL
In a structural sense, much
attention has been directed toward
use of cupronickel or cupronickel clad
steel in the hulls of small shrimp
treats(L6). Economic analysis of use
~f either sheathing or integrally
“=nded clad in large containerships
xas shcwn some advantages, but as yet
>0 large ships have been built.
Emphasis has been placed on the
properties which, in extreme load
environments , will contribute to hull
integrity, or in their absence, to
Despite an i“tensi”e research
and development program over 35 years,
more work remains ahead.
the weldability of medium strength
hull steels is of high priority and
is moving ahead at a good rate.
An experimental rudder was i“stalled on the westward venture, a 26
knot Ro-Ro for the evaluation of
cupronicke 1 sheathing.
~ate has bee” satisfactory (Figure 27) .
Cent in”ed coope ratio” between
naval architects, materials producers,
regulatory agencies and shipbuilders
will insure prcqress toward o“r
common goal of improving ship hull
Rules for Building and
Classing steel Vessels (Annual)
ABS Rules for Building and
Classing Aluminum Vessels (1975)
ABS Rules for Building and
Classing Steel Barges for Offshore
ABS RUleS for Building and
Classing Steel Floating Dry
ABS RUle S for Building and
Classinq Underwater Systems and
ABS Rules for Building and
Classing Bulk Carriers for Ser”ice
on the GIeat Lakes (1978)
API specification 2H ‘,
Offshore Drilling Rigs”
SR-Project 1256--In”estigation of
Steels for lmpro”ed Weldability
High performance submersibles
ha”e used titanium in their hull
Alvi”” , originally fitted
with a“ HY1OO pressure hull, has bee”
reconstructed with a titanium alloy
However, no commercial “essels
use titanium in hull components.
1980, Part 4
This survey of the current state
of the art is intended to provide an
o“erview of the available materials
for ship hull construction.
will “ot permit more than a brief
discussion of tbe critical factors
which affect hull performance under
Effect of Weld Defects - SRC
Hawthorne, J. R. and Loss, F. J.
“Fracture Toughness Characterization of Shipbuilding Steel s,,SSC
248, 1975, Washington
Rolfe, S. T., Rhea, D. M. and
Kuzmanovic, B. O. “Fracture
Control Guidelines for Welded
Steel Ship Hulls,, SRC 244,
Pellini, W. S. and P“zak, P. P.
“Fracture Analysis Diagram Procedures for the Fracture-Safe
Engineering Design of Steel
Structures’, USNRL Report 5920
Pense , A . W. ‘sE”aluation of
Fracture Criteria for Ship Steels
Plus Weldments,, SR 1265, Report
Wilson, A. D. “The Fatiy”e and
Toughness Properties of a C-Mn-Cb
Plate Steel,, ASME Journal of
Engineering Materials and Technology, Volume 102, July, 1980
Prager, M. and Thiele, E. W.
“Welding a Copper Nickel Clad
Ship - Copper Mariner 11”,
Welding Journal, volume 59,
No. 7, July 1979 a“d Manzolillo,
J. L., Thiele, E. W. and T“thill,
A. H. CA-706 Copper Nickel Alloy
The Copper Marine
Experience & Economics -- Pre sented at SNAME Annual Meeting